This specification covers two grades of electric-resistance-welded steel pipe intended for conveying gas, vapor, water or other liquid. The steel shall be made by either or both basic-oxygen or electric-furnace processes. Steel may be cast in ingots or may be strand cast. The pipe shall be manufactured from flat rolled steel in individual lengths or continuous length by electric-resistance or electric-induction welding without the addition of extraneous material. The weld seam of electric-resistance welded pipe to Grade B pipe shall be heat treated after welding or processed in such a manner that no untempered martensite remains. Tensile and chemical requirements of the steel are provided. Specimens of the steel pipes are subject to flattening test and hydrostatic test. A nondestructive electric test, either electromagnetic (eddy current) or ultrasonic test, may be preferred as an alternate to the hydrostatic test.

This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.

1. Scope

1.1 This specification2 covers two grades of electric-resistance-welded steel pipe in NPS 2 to NPS 30 [DN 50 to DN 750] inclusive, with nominal (average) wall thickness up to 0.500 in. [12.70 mm], inclusive, and in nominal sizes NPS 3/4 to NPS 5 [DN 20 to DN 125] inclusive with nominal (average) wall thickness 0.083 in. [2.11 mm] to 0.134 in. [3.40 mm], depending on size. Pipe having other dimensions (Note 1) may be furnished provided such pipe complies with all other requirements of this specification. The pipe is intended for conveying gas, vapor, water or other liquid; only Grade A is adapted for flanging and bending (Note 2). The suitability of pipe for various purposes is somewhat dependent upon its dimensions, properties, and conditions of service, so that the purpose for which the pipe is intended should be stated in the order. The pipe may be furnished either nonexpanded or cold expanded at the option of the manufacturer. When pipe is cold expanded, the amount of expansion shall not exceed 1.5 % of the outside diameter pipe size.

Note 2—This provision is not intended to prohibit the cold bending of Grade B pipe.

1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.